# Hot Rolled (+U) 1.0314 Steel

EN 1.0314 +U steel is EN 1.0314 steel in the hot worked condition. The graph bars on the material properties cards below compare EN 1.0314 +U steel to: wrought carbon or non-alloy steels (top), all iron alloys (middle), and the entire database (bottom). A full bar means this is the highest value in the relevant set. A half-full bar means it's 50% of the highest, and so on.

## Mechanical Properties

Brinell Hardness

92

Elastic (Young's, Tensile) Modulus

190 *GPa* 27 *x 10 ^{6} psi*

Elongation at Break

25 *%*

Fatigue Strength

140 *MPa* 20 *x 10 ^{3} psi*

Poisson's Ratio

0.29

Reduction in Area

86 *%*

Shear Modulus

73 *GPa* 11 *x 10 ^{6} psi*

Shear Strength

200 *MPa* 29 *x 10 ^{3} psi*

Tensile Strength: Ultimate (UTS)

320 *MPa* 46 *x 10 ^{3} psi*

Tensile Strength: Yield (Proof)

190 *MPa* 27 *x 10 ^{3} psi*

## Thermal Properties

Latent Heat of Fusion

250 *J/g*

Maximum Temperature: Mechanical

400 *°C* 750 *°F*

Melting Completion (Liquidus)

1470 *°C* 2670 *°F*

Melting Onset (Solidus)

1430 *°C* 2600 *°F*

Specific Heat Capacity

470 *J/kg-K* 0.11 *BTU/lb-°F*

Thermal Conductivity

53 *W/m-K* 30 *BTU/h-ft-°F*

Thermal Expansion

12 *µm/m-K*

## Electrical Properties

Electrical Conductivity: Equal Volume

6.9 *% IACS*

Electrical Conductivity: Equal Weight (Specific)

7.9 *% IACS*

## Otherwise Unclassified Properties

Base Metal Price

1.8 *% relative*

Density

7.9 *g/cm ^{3}* 490

*lb/ft*

^{3}Embodied Carbon

1.4 *kg CO _{2}/kg material*

Embodied Energy

18 *MJ/kg* 7.8 *x 10 ^{3} BTU/lb*

Embodied Water

46 *L/kg* 5.4 *gal/lb*

## Common Calculations

Resilience: Ultimate (Unit Rupture Work)

68 *MJ/m ^{3}*

Resilience: Unit (Modulus of Resilience)

95 *kJ/m ^{3}*

Stiffness to Weight: Axial

13 *points*

Stiffness to Weight: Bending

24 *points*

Strength to Weight: Axial

11 *points*

Strength to Weight: Bending

13 *points*

Thermal Diffusivity

14 *mm ^{2}/s*

Thermal Shock Resistance

10 *points*

## Alloy Composition

Fe | 99.365 to 99.78 | |

Mn | 0.2 to 0.4 | |

Si | 0 to 0.1 | |

Al | 0.020 to 0.060 | |

C | 0 to 0.030 | |

S | 0 to 0.025 | |

P | 0 to 0.020 |

All values are % weight. Ranges represent what is permitted under applicable standards.

## Followup Questions

## Further Reading

EN 10263-2: Steel rod, bars and wire for cold heading and cold extrusion - Part 2: Technical delivery conditions for steels not intended for heat treatment after cold working

Carbon Steel Handbook, D. Gandy, 2007

Ferrous Materials: Steel and Cast Iron, Hans Berns and Werner Theisen, 2008

Steels: Processing, Structure, and Performance, 2nd ed., George Krauss, 2015